Presentation on theme: "The hot dip galvanizing process"— Presentation transcript:
1 The hot dip galvanizing process Technical seminar
2 The hot dip galvanizing process Loading - jiggingDegreasingHot causticPicklingHydrochloric acidPre-fluxingZinc am. chlorideHot dip galvanizingMolten zincQuenchingDichromate
3 The hot dip galvanizing process Loading - jiggingThe steel items need to be supported during the hot dip galvanizing process.Can the item be easily jigged?Will touch marks be a problem?Solutions and molten zinc must be able to flow into all sections and drain off all sections.Steel items must be designed to prevent air, solutions and molten zinc becoming trappedCheck design for possible problems
4 The hot dip galvanizing process DegreasingA hot (90oC) caustic bath is used to remove -Oil, grease, paint another organic compoundsIf these contaminating materials are not removed, the next stage of the process (pickling) is affectedCheck if any paint is on item - some paints are not easily removed and may require abrasive blasting before galvanizingSome pipes and pipe fittings have a black varnish coating that cannot be removed in the caustic bath.
5 The hot dip galvanizing process Acid picklingThe steel items are immersed in hydrochloric acid to remove - rust, mill scale and other metal oxidesThe steel surface must be perfectly clean of these oxides for the molten zinc to react with the steelVery heavy rust may not be easily removed by pickling - badly rusted items should be abrasive blasted or mechanically cleaned first.
6 The hot dip galvanizing process Pre-fluxingSteel items are water rinsed after pickling and immersed in hot (70-80oC) zinc ammonium chloride (ZAC) solution.The ZAC solution conditions the clean steel surface ready for hot dip galvanizing.Good pre-treatment = good quality galvanizing
7 The hot dip galvanizing process QuenchingAfter hot dip galvanized steel item is removed from the galvanizing bath, it is immediately quenched in a sodium dichromate solutionThe dichromate quenching cools the item so that it can be quickly handled and passivates the surface of the galvanized coating to maintain its bright appearance.
8 The hot dip galvanizing process The steel is immersed in molten zinc (temp 4500C)The clean steel surface reacts with the molten zinc to form a zinc-iron alloy which is very strongly bonded to the surface.The hot dip galvanized coating forms in 3-5 minutes, depending on the steel thickness.Free zinc layerGalvanized coatingAlloy layersSteelMicrograph X
9 The hot dip galvanizing process QuenchingAfter hot dip galvanized steel item is removed from the galvanizing bath, it is immediately quenched in a sodium dichromate solutionThe dichromate quenching cools the item so that it can be quickly handled and conditions the surface of the galvanized coating to maintain its bright appearance.Dichromate quenching will reduce white rusting problems. White rust forms when rainwater reacts with newly galvanized steel to form zinc hydroxide.Poor storage or HDG steel will also promote white rust.
10 The hot dip galvanizing process CharacteristicsTypically microns thick ( 1 mm = 1000 microns)Zinc iron alloy layers make up 80% % of the coating.The zinc-iron alloy layers are harder than 250 grade steelSteelZinc-iron alloysZincMicrograph of hot dip galvanized coating
11 The hot dip galvanizing process Coating comparisonsCompared to zinc electroplating (ZEP)and continuous galvanizing (CG), hot dip galvanizing (HDG) is better because…..- HDG is thicker and will last over 50 years or more without rusting- HDG is harder and is 5 times more abrasion resistant than ZEP and CG- HDG coats all external and internal surfaces and edges. All CG coatings have cut, exposed edges after processing.
12 Coating thickness of coatings on galvanized products Z350 Gal. sheetHDG HeavyCoating thickness - micronsElectroplatingHDG Light
13 The hot dip galvanizing process Zinc cost versus surface area versus zinc pickupZinc price 2.00/kgGood design reduces excessive zinc pick-up